3 Fracture ModesSimple fracture is the separation of a body into 2 or more pieces in response to an applied stress that is static (constant) and at temperatures that are low relative to the Tm of the material.Classification is based on the ability of a material to experience plastic deformation.Ductile fractureAccompanied by significant plastic deformationBrittle fractureLittle or no plastic deformationSudden, catastrophic33
4 Fracture Mechanism Imposed stress Crack Formation Propagation Ductile failure has extensive plastic deformation in the vicinity of the advancing crack. The process proceeds relatively slow (stable). The crack resists any further extension unless there is an increase in the applied stress.In brittle failure, cracks may spread very rapidly, with little deformation. These cracks are more unstable and crack propagation will continue without an increase in the applied stress.
5 Crack Propagation Cracks propagate due to sharpness of crack tip A plastic material deforms at the tip, “blunting” the crack.deformed regionbrittleEnergy balance on the crackElastic strain energy-energy stored in material as it is elastically deformedthis energy is released when the crack propagatescreation of new surfaces requires energyplastic555
6 Ductile vs Brittle Failure VeryDuctileModeratelyBrittleFracturebehavior:LargeModerate%AR or %ELSmall• Ductile fracture isusually more desirablethan brittle fracture.Ductile:Warning before fractureBrittle: No warning6
7 Moderately Ductile Failure • Evolution to failure:voidnucleationCoalescenceof cavitiesCrackpropagationfracturenecking• Resultingfracturesurfaces(steel)50 mmparticlesserve as voidnucleationsites.From V.J. Colangelo and F.A. Heiser, Analysis of Metallurgical Failures (2nd ed.), Fig , p. 294, John Wiley and Sons, Inc., (Orig. source: P. Thornton, J. Mater. Sci., Vol. 6, 1971, pp )100 mmFracture surface of tire cord wire loaded in tension. Courtesy of F. Roehrig, CC Technologies, Dublin, OH. Used with permission.77
8 Example: Pipe Failures • Ductile failure:-- one piece-- large deformation• Brittle failure:-- many pieces-- small deformationsFigures from V.J. Colangelo and F.A. Heiser, Analysis of Metallurgical Failures (2nd ed.), Fig. 4.1(a) and (b), p. 66 John Wiley and Sons, Inc., Used with permission.88
9 Ductile vs. Brittle Failure c09f03abDuctile vs. Brittle Failurecup-and-cone fracturebrittle fracture
10 c09f04Ductile Failure(a) SEM image showing spherical dimples resulting from a uniaxial tensile load. (b) SEM image of parabolic dimples from shear loading.
11 Brittle FractureArrows indicate point at failure originationDistinctive pattern on the fracture surface: V-shaped “chevron” markings point to the failure origin.1111
12 Transgranular Fracture c09f06abTransgranular FractureCleavage - in most brittle crystalline materials, crack propagation that results from the repeated breaking of atomic bonds along specific planes.This leads to transgranular fracture where the crack splits (cleaves) through the grains.
13 Intergranular Fracture c09f07abIntergranular failure is typically due to elemental depletion (chromium) at the grain boundaries or some type of weakening of the grain boundary due to chemical attack, oxidation, embrittlement.
15 Stress ConcentrationThe measured fracture strengths for most brittle materials are significantly lower than those predicted by theoretical calculations based on atomic bond energies.This discrepancy is explained by the presence of very small, microscopic flaws or cracks that are inherent to the material.The flaws act as stress concentrators or stress raisers, amplifying the stress at a given point.This localized stress diminishes with distance away from the crack tip.
16 Fracture ToughnessFracture toughness measures a material’s resistance to brittle fracture when a crack is present.It is an indication of the amount of stress required to propagate a preexisting flaw.Flaws may appear as cracks, voids, metallurgical inclusions, weld defects, design discontinuities, or some combination thereof.It is common practice to assume that flaws are present and use the linear elastic fracture mechanics (LEFM) approach to design critical components.This approach uses the flaw size and features, component geometry, loading conditions and the fracture toughness to evaluate the ability of a component containing a flaw to resist fracture.
17 Ductile vs BrittleThe effect of a stress raiser is more significant in brittle than in ductile materials.For a ductile material, plastic deformation results when the maximum stress exceeds the yield strength.This leads to a more uniform distribution of stress in the vicinity of the stress raiser; the maximum stress concentration factor will be less than the theoretical value.In brittle materials, there is no redistribution or yielding.
19 stress-intensity factor (K) The stress-intensity factor (K) is used to determine the fracture toughness of most materials.A Roman numeral subscript indicates the mode of fracture and the three modes of fracture are illustrated in the image to the right.Mode I fracture is the condition where the crack plane is normal to the direction of largest tensile loading. This is the most commonly encountered mode.The stress intensity factor is a function of loading, crack size, and structural geometry. The stress intensity factor may be represented by the following equation:KI is the fracture toughness in σ is the applied stress in MPa or psia is the crack length in meters or inches is a crack length and component geometry factor that is different for each specimen, dimensionless.
20 Fracture toughness - good diagrams Critical StressAll brittle materials contain a population of small cracks and flaws that have a variety of sizes, geometries and orientations.When the magnitude of a tensile stress at the tip of one of these flaws exceeds the value of this critical stress, a crack forms and then propagates, leading to failure.Condition for crack propagation:K ≥ KcStress Intensity Factor:--Depends on load & geometry.Fracture Toughness:--Depends on the material,temperature, environment &rate of loading.Fracture toughness - good diagrams
21 Compact tension (CT) specimen single edge notch bend (SENB or three-point bend)
22 Flaws are Stress Concentrators If the crack is similar to an elliptical hole through plate, and is oriented perpendicular to applied stress, the maximum stress σm=where t = radius of curvatureso = applied stresssm = stress at crack tipa = length of surface crack or ½ length of internal cracksm / so = Kt the stress concentration factortStress concentrated at crack tip22
23 DESIGN AGAINST CRACK GROWTH • Crack growth condition:K ≥ Kc• Largest, most stressed cracks grow first.--Result 1: Max flaw sizedictates design stress.--Result 2: Design stressdictates max. flaw size.
24 Design Example: Aircraft Wing • Material has Kc = 26 MPa-m0.5• Two designs to consider...Design A-- largest flaw is 9 mm-- failure stress = 112 MPaDesign B-- use same material-- largest flaw is 4 mm-- failure stress = ?• Use...• Key point: Y and Kc are the same in both designs. Y is a dimensionless parameter; see Callister page 298.9 mm112 MPa4 mm-- Result:Answer:• Reducing flaw size pays off.2424
25 Sensors made to mesh with plane Structural engineers have long imagined the day when materials used in an aircraft, a wind turbine blade or a bridge could sense if they had been strained to the point of damage, reducing their load-carrying capacity, and report that information in real time before the structure's safety is compromised.For many years, such a scenario was more the stuff of science fiction than fact, but today, structural health monitoring (SHM) systems that can perform these tasks are closer to reality.Scientists have created a fiber mesh embedded with sensors designed to monitor an airplane’s structural integrity and outside temperature.When wrapped around an aircraft, the sensors could help prevent microscopic cracks from developing into catastrophic failures.Made from a plastic polymer, the mesh is designed so it doesn’t add significant weight or drag to an aircraft.The technology also could be used in autos, packaging and medical devices.
26 A piezoelectric-based sensor system from Acellent Technologies, called SMART Layer, identifies damage with small ceramic actuatorsStructural health monitoring (SHM) systems can be arrayed in similar fashion to the human nervous system, with sensors concentrated in key areas where loads are highest.An FAA-sponsored study on curved honeycomb-cored panels showed that acoustic emission (AE) monitoring is a reliable method for locating damage initiation sites and for tracking crack progression. Source: Physical Acoustics CorpA comparative vacuum-monitoring (CVM) sensor, is a thin, self-adhesive rubber patch that detects cracks in the underlying material. The rubber is laser-etched with rows of tiny, interconnected channels or galleries, to which an air pressure is applied. Any propagating crack under the sensor breaches the galleries and the resulting change in pressure is monitored.
28 Brittle Fracture of Ceramics c09f13Most ceramics (at room temperature) fracture before any plastic deformation can occur.Typical crack configurations for 4 common loading methods.
29 Brittle Fracture of Ceramics Surface of a 6-mm diameter fused silica rod.Characteristic fracture behavior in ceramicsOrigin pointInitial region (mirror) is flat and smoothAfter reaches critical velocity crack branchesmisthackle2929
30 Fracture of PolymersThe fracture strengths of polymers are low relative to ceramics and metals.The fracture mode in thermosetting polymers (heavily crosslinked networks) is typically brittle.For thermoplastic polymers, both ductile and brittle modes are possible. Reduced temperature, increased strain rate, sharp notches, increased specimen thickness are some factors that can influence a brittle fracture.One phenomenon that occurs in thermoplastics is crazing, very localized plastic deformation and formation of microvoids and fibrillar bridgesfibrillar bridgesmicrovoidscrackaligned chainsNote: crack spreads by breaking C-C bondsDuctile plastics have large craze zones that absorb large amounts of energy as it spreads303030
31 Impact Testing • Impact loading: -- severe testing case -- makes material more brittle-- decreases toughness(Charpy)final heightinitial height3131
32 Ductile to Brittle Transition Temperature (DBTT) • Pre-WWII: The Titanic• WWII: Liberty shipsDisastrous consequences for a welded transport ship, suddenly split across the entire girth of the ship (40˚F). The vessels were constructed from steel alloys that exhibit a DBTT room tempReprinted w/ permission from R.W. Hertzberg, "Deformation and Fracture Mechanics of Engineering Materials", (4th ed.) Fig. 7.1(a), p. 262, John Wiley and Sons, Inc., (Orig. source: Dr. Robert D. Ballard, The Discovery of the Titanic.)3232
33 Charpy Impact Energy (A) and Shear Fracture % (B) Correlated with Temperature c09f19
34 c09f20 Steel Charpy Samples Fracture surfaces after impact showing the variation in ductility with testing temperature (˚C).
35 Temperature • Increasing temperature... -- increases %EL and Kc• Ductile-to-Brittle Transition Temperature (DBTT)...FCC metals (e.g., Cu, Ni)BCC metals (e.g., iron at T < 914°C)polymersImpact EnergyBrittleMore DuctileHigh strength materials (sy> E/150)TemperatureDuctile-to-brittletransition temperature3535
36 Fatiguec09f24Fatigue testing apparatus for rotating bending testFatigue is a form of failure that occurs in structures subjected to dynamic stresses over an extended period.Under these conditions it is possible to fail at stress levels considerably lower than tensile or yield strength for a static load.Single largest cause of failure in metals; also affects polymers and ceramics.Common failure in bridges, aircraft and machine components.
37 Cyclic Stress - Fatigue c09f23Variation of stress with time that accounts for fatigue failures.The stress may be axial (tension-compression), flexural (bending) or torsional (twisting) in nature.There are 3 fluctuating stress-time modes seen in the figure: (a) reversed stress cycle - symmetrical amplitude about a mean zero stress level; (b) repeated stress cycle - asymmetrical maxima and minima relative to the zero stress level; (c) variable (random) stress level
38 Fatiguec09f30Fracture surface with crack initiation at top. Surface shows predominantly dull fibrous texture where rapid failure occurred after crack achieved critical size.Fatigue failureCrack initiationCrack propagationFinal failure
39 Striations are close together indicating low stress, many cycles. Widely spaced striations mean high stress few cycles.c09f29Fatigue failure is brittle in nature, even in normally ductile materials; there is very little plastic deformation associated with the failure.The image shows fatigue striations (microscopic).
40 Federal investigators say metal fatigue caused a hole to rip open in the roof of a Southwest Airlines jet as it cruised at 35,000 feet last year (2009). The National Transportation Safety Board says the 14-inch crack developed in a spot where two sheets of aluminum skin were bonded together on the Boeing 737 jet.The pilot made an emergency landing in Charleston, W.Va. There were no injuries among the 126 passengers and five crew members. Two months after the scare, Boeing told all airlines with 737s to conduct repeated inspections of the top of the fuselage near the vertical tail fin. The Federal Aviation Administration has since made those inspections mandatory.Southwest got the plane in 1994 — it's much older than the average Southwest jet — and had flown it for 50,500 hours and made 42,500 takeoffs and landings before it sprang a hole in the roof, according to the safety board report. The safety board said it found signs of metal fatigue by magnifying the area in front of the tail fin. In a 3-inch stretch, the crack penetrated completely through the aluminum skin.FAA records showed that eight cracks had been found and repaired in the fuselage during the plane's 14-year checkup.
41 Fatigue Mechanism • Crack grows incrementally • Failed rotating shaft typ. 1 to 6increase in crack length per loading cyclecrack origin• Failed rotating shaft-- crack grew even thoughKmax < Kc-- crack grows faster as• Ds increases• crack gets longer• loading freq. increases.Adapted fromFig. 9.28, Callister & Rethwisch 3e. (Fig is from D.J. Wulpi, Understanding How Components Fail, American Society for Metals, Materials Park, OH, 1985.)41
42 Crack growth rateInitially, growth rate is small, but increases with increasing crack length.Growth rate increases with applied stress level for a given crack length (a1).
43 S-N Curvesc09f25A specimen is subjected to stress cycling at a maximum stress amplitude; the number of cycles to failure is determined.This procedure is repeated on other specimens at progressively decreasing stress amplitudes.Data are plotted as stress S versus number N of cycles to failure for all the specimen.Typical S-N behavior: the higher the stress level, the fewer the number of cycles.
44 Fatigue Limitc09f25For some iron and titanium alloys, the S-N curve becomes horizontal at higher number of cycles N.Essentially it has reached a fatigue limit, and below this stress level the material will not fatigue.The fatigue limit represents the largest value of fluctuating stress that will not cause failure for an infinite number of cycles.
46 c09f33Surface TreatmentsDuring machining operations, small scratches and grooves can be introduced; these can limit the fatigue life.Improving the surface finish by polishing will enhance fatigue life significantly.One of the most effective methods of increasing fatigue performance is by imposing residual compressive stresses within a thin outer surface layer. A surface tensile stress will be offset by the compressive stress.Shot peening (localized plastic deformation) with small (diameters ranging from 0.1 to 1.0 mm), hard particles (shot) are projected at high velocities on to the surface. The resulting deformation induces compressive stresses to a depth of roughly ¼ to ½ of the shot diameter.The influence of shot peening is compared in the graph.
47 Improving Fatigue Life 1. Impose a compressive surface stress(to suppress surface cracks from growing)--Method 1: shot peeningputsurfaceintocompressionshot--Method 2: carburizingC-rich gas2. Remove stressconcentrators.badbetter
48 Case Hardeningc09f34Case hardening is a technique where both surface hardness and fatigue life are improved for steel alloys.Both core region and carburized outer case region are seen in image. Knoop microhardness shows case has higher hardness (smaller indent).A carbon or nitrogen rich outer surface layer (case) is introduced by atomic diffusion from the gaseous phase. The case is typically 1mm deep and is harder than the inner core material.
50 CreepMaterials are often placed in service at elevated temperatures (>0.4 Tm) and exposed to static mechanical stresses.Examples are turbine rotors in jet engines and steam generators that experience centrifugal stresses and high pressure steam lines.Creep is time dependent, permanent deformation of the material when subjected to a constant load or stress.
51 Creepc09f35A typical creep test consists of subjecting a specimen to a constant load or stress while maintaining constant temperature.Upon loading, there is instant elastic deformation. The resulting creep curve consists of 3 regions: primary or transient creep adjusts to the creep level (creep rate may decrease); secondary creep-steady state-constant creep rate, fairly linear region (strain hardening and recovery stage); tertiary creep, there is accelerated rate of strain until rupture (grain boundary separation, internal crack formation, cavities and voids).Creep strain vs time at constant load and constant elevated temperature. Minimum creep rate (steady-state creep rate), is the slope of the linear segment in the secondary region. Rupture lifetime tr is the total time to rupture.
52 Creep Sample deformation at a constant stress (s) vs. time s s,e tPrimary Creep: slope (creep rate) decreases with time.Secondary Creep: steady-state i.e., constant slope.Tertiary Creep: slope (creep rate) increases with time, i.e. acceleration of rate.
54 Creepc09f37Dependence of creep strain rate on stress; stress versus rupture lifetime for a low carbon-nickel alloy at 3 temperatures.
55 Secondary Creep • Strain rate is constant at a given T, s -- strain hardening is balanced by recoverystress exponent (material parameter)activation energy for creep(material parameter)strain ratematerial const.applied stress• Strain rateincreasesfor higher T, s1024-2-11Steady state creep rate (%/1000hr)esStress (MPa)427°C538°C64955
56 SUMMARY • Engineering materials don't reach theoretical strength. • Flaws produce stress concentrations that causepremature failure.• Sharp corners produce large stress concentrationsand premature failure.• Failure type depends on T and stress:- for noncyclic s and T < 0.4Tm, failure stress decreases with:- increased maximum flaw size,- decreased T,- increased rate of loading.- for cyclic s:- cycles to fail decreases as Ds increases.- for higher T (T > 0.4Tm):- time to fail decreases as s or T increases.56